/ Home / About the University / University structure / Faculties / Faculty of Science and Engineering / Electron Microscopy Centre / Scarlet PL case study
Scarlet PL case study
Case study highlighting how the Plymouth Materials Characterisation Project (PMCP) has benefited Scarlet PL
; What is FIB-SEM?
Contact the Plymouth Electron Microscopy Centre on emc@plymouth.ac.uk or Claire Pearce, Project Manager, directly.
You can also call the PEMC team on +44 1752 588908
Scarlet PL, based in Plymouth, design and manufacture an instrument containing various sensors, that is used deep in oil and gas wells for monitoring purposes and with the aim of extending the life of the wells. With market opportunities in the US, Saudi Arabia and Indonesia, Scarlet PL is keen to perfect the product, including understanding the causes of failure at the end of the product life. In addition, it is key to understand the metallurgy of the weld used in the product, so that when production reaches high numbers, the best techniques and equipment are in use.
What did they want?
Currently Scarlet PL outsource their laser welding and would like to begin laser welding in-house. They want to have their welding analysed to check the quality of the weld and to understand the metallurgy of the weld in order to ensure it supports high production numbers for the new product.
Agreed analysis plan
The welded part had two parts of the same weld in view and it was agreed that both welds would be analysed using electron backscatter diffraction (EBSD), which is a technique used to analyse grain structure. If there was anything of interest in either/both of the welds, then further analysis will be carried out at a higher resolution.
Initial results
The right-hand weld was analysed first and it was observed to be of good quality with no visible defects, as shown in the top EBSD map. It was observed that there was good interface between the weld and the parent material with the grains in the parent material 'blending' into the weld. The centre of the weld had more equiaxed grains which would indicate recrystallisation due to the centre being exposed to higher temperatures.
The left-hand weld was observed to have two cracks at the interface either side of the weld, as shown in the bottom of the EBSD map. Much like with the right-hand weld the grains of the parent material at the interface have 'blended' into the weld with recrystallisation occurring in the centre of the weld, although it would appear that a higher degree of recrystallisation may have occurred. Subsequently a new EBSD map was acquired over the area of both cracks, using a higher pixel resolution.
Further results
It was observed that the right-hand crack seems to be connected to a void at the interface that then split and propagated on either side of the void, whereas the left-hand crack was not associated with a void and purely cracked along the interface. It was also observed that along both cracks there was a high number of very fine grains which would have been due to recrystallisation under high stress; this was also observed at the bottom of the void. The grains that show a mottling effect (multiple colours) are grains that are under a high amount stress and colour comes from a misorientation in the crystal structure. These mottled grains could split and form much smaller grains, which most likely was what happened along the crack to form the fine grain structure.
TKD and STEM-EDS analysis
Transmission kikuchi diffraction (TKD) and scanning tranmission electron microscopy (STEM) EDS were carried out on a thin lamella section taken from parallel to the left crack on the side of the parent material; this was to analyse the nano-grain structure at the crack. A large grain was observed in the TKD map (top right corner) which was shown to have a large amount of stress. This grain may be the original grain that 'split' to form the much smaller grains shown in the rest of the map. This may suggest that the large grains at the crack that were highly stressed, recrystallised to form this nano-grain structure. The STEM-EDS showed an area with low concentrations of nickel (Ni) and chromium (Cr) and high concentrations of niobium (Nb) and titanium (Ti). This may be the formation of a niobium-titanium-carbide, this formation of carbides may cause cracking as carbides are inherently brittle.
Also in Electron Microscopy Centre
3D reconstruction of porous materials through FIB-SEM
ARC Marine Case Study
Cathodoluminescence
Composite Innovations Ltd case study
Cryo-Scanning Electron Microscopy
DavyJ Ltd Case Study
Dynamics of formation and secretion of heterococcoliths by Coccolithus pelagicus
Electron Backscatter Diffraction (EBSD)
Energy Dispersive Spectroscopy (EDS)
Enigma Audio Case Study
Esterlam International Ltd case study
Facilities at Plymouth Electron Microscopy Centre
FIB-SEM: Under the hood
Focused Ion Beam
Gas Injection System (GIS)
Hunting for meteorites in the Nullarbor Plain
Industrial Case Studies
JEOL 1400 TEM
JEOL 6610 LV SEM
JEOL 7001 FE SEM
Large Area Mapping
Low Vacuum Mode (variable pressure)
Low Voltage - Scanning Transmission Electron Microscopy (LV-STEM)
Low Voltage-STEM vs TEM
Microscopic study of (assemblies of) nano-objects
Owens Case Study
PEMC equipment
PEMC sample preparation
PEMC techniques
Plessey Semiconductors Ltd case one
Plessey Semiconductors Ltd case study
Plessey Semiconductors Ltd case three
Plessey Semiconductors Ltd case two
Plymouth Electron Microscopy Centre news and events
Plymouth Materials Characterisation Project (PMCP)
PML Applications Ltd Case Study
Radley Scientific case study
Ramer Sponges Ltd Case Study
Scanning Electron Microscopy (SEM)
Schools liaison and outreach
Serial Sectioning Tomography
South West Metal Finishing Case Study
TEM Tomography
Testing the Capabilities of Automated Mineralogy in Mining
The Effect of Different Post-Electroplating Surface Modification Treatments on Tin Whisker Growth
Thin section lift-out
ZEISS Crossbeam 550 FIB-SEM